StressStrain Behavior


 Joel Horton
 1 years ago
 Views:
Transcription
1 StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation. Calculate the resulting strain. This problem calls for us to calculate the elastic strain that results for an aluminum specimen stressed in tension. The crosssectional area is just (10 mm) (1.7 mm) 17 mm ( m 0.0 in. ); also, the elastic modulus for Al is given in Table 6.1 as 69 GPa (or N/m ). Combining Equations 6.1 and 6.5 and solving for the strain yields ε σ E F A 0 E 35,500 N ( m )( N/m ) 6.5 A steel bar 100 mm (4.0 in.) long and having a square cross section 0 mm (0.8 in.) on an edge is pulled in tension with a load of 89,000 N (0,000 lb f ), and experiences an elongation of 0.10 mm ( in.). Assuming that the deformation is entirely elastic, calculate the elastic modulus of the steel. This problem asks us to compute the elastic modulus of steel. For a square crosssection, A 0 b 0, where b 0 is the edge length. Combining Equations 6.1, 6., and 6.5 and solving for E, leads to F E σ ε A 0 l F b 0 l (89,000 N)( m) ( m) ( m) N/m 3 GPa ( psi)
2 6.7 For a bronze alloy, the stress at which plastic deformation begins is 75 MPa (40,000 psi), and the modulus of elasticity is 115 GPa ( psi). (a) What is the maximum load that may be applied to a specimen with a crosssectional area of 35 mm (0.5 in. ) without plastic deformation? (b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to which it may be stretched without causing plastic deformation? (a) This portion of the problem calls for a determination of the maximum load that can be applied without plastic deformation (F y ). Taking the yield strength to be 75 MPa, and employment of Equation 6.1 leads to F y σ y A 0 ( N/m )( m ) 89,375 N (0,000 lb f ) (b) The maximum length to which the sample may be deformed without plastic deformation is determined from Equations 6. and 6.5 as l i 1 + σ E 75 MPa (115 mm) mm (4.51 in.) MPa Elastic Properties of Materials 6.15 A cylindrical specimen of aluminum having a diameter of 19 mm (0.75 in.) and length of 00 mm (8.0 in.) is deformed elastically in tension with a force of 48,800 N (11,000 lb f ). Using the data contained in Table 6.1, determine the following: (a) The amount by which this specimen will elongate in the direction of the applied stress. (b) The change in diameter of the specimen. Will the diameter increase or decrease?
3 (a) We are asked, in this portion of the problem, to determine the elongation of a cylindrical specimen of aluminum. Combining Equations 6.1, 6., and 6.5, leads to F π d 0 4 σ Eε E l Or, solving for l (and realizing that E 69 GPa, Table 6.1), yields l 4F π d 0 E (4)(48,800 N)( m) (π)( m) ( N /m ) m 0.50 mm (0.0 in.) (b) We are now called upon to determine the change in diameter, d. Using Equation 6.8 ν ε x ε z d / d 0 l / From Table 6.1, for aluminum, ν Now, solving the above expression for d yields d ν l d 0 (0.33)(0.50 mm)(19 mm) 00 mm mm ( in.) The diameter will decrease A cylindrical specimen of a hypothetical metal alloy is stressed in compression. If its original and final diameters are and 0.05 mm, respectively, and its final length is mm, compute its original length if the deformation is totally elastic. The elastic and shear moduli for this alloy are 105 GPa and 39.7 GPa, respectively.
4 This problem asks that we compute the original length of a cylindrical specimen that is stressed in compression. It is first convenient to compute the lateral strain ε x as ε x d 0.05 mm mm d mm In order to determine the longitudinal strain ε z we need Poisson's ratio, which may be computed using Equation 6.9; solving for ν yields ν E G MPa ()( MPa) Now ε z may be computed from Equation 6.8 as ε z ε x ν Now solving for using Equation 6. l i 1 + ε z mm 75.5 mm A brass alloy is known to have a yield strength of 75 MPa (40,000 psi), a tensile strength of 380 MPa (55,000 psi), and an elastic modulus of 103 GPa ( psi). A cylindrical specimen of this alloy 1.7 mm (0.50 in.) in diameter and 50 mm (10.0 in.) long is stressed in tension and found to elongate 7.6 mm (0.30 in.). On the basis of the information given, is it possible to compute the magnitude of the load that is necessary to produce this change in length? If so, calculate the load. If not, explain why. We are asked to ascertain whether or not it is possible to compute, for brass, the magnitude of the load necessary to produce an elongation of 7.6 mm (0.30 in.). It is first necessary to compute the strain at yielding from the yield strength and the elastic modulus, and then the strain experienced by the test specimen. Then, if
5 ε(test) < ε(yield) deformation is elastic, and the load may be computed using Equations 6.1 and 6.5. However, if ε(test) > ε(yield) computation of the load is not possible inasmuch as deformation is plastic and we have neither a stressstrain plot nor a mathematical expression relating plastic stress and strain. We compute these two strain values as ε(test) l 7.6 mm 50 mm 0.03 and ε(yield) σ y E 75 MPa MPa Therefore, computation of the load is not possible since ε(test) > ε(yield). Tensile Properties 6.5 Figure 6.1 shows the tensile engineering stress strain behavior for a steel alloy. (a) What is the modulus of elasticity? (b) What is the proportional limit? (c) What is the yield strength at a strain offset of 0.00? (d) What is the tensile strength? Using the stressstrain plot for a steel alloy (Figure 6.1), we are asked to determine several of its mechanical characteristics. (a) The elastic modulus is just the slope of the initial linear portion of the curve; or, from the inset and using Equation 6.10 E σ σ 1 ε ε 1 (00 0) MPa ( ) MPa 00 GPa ( psi) The value given in Table 6.1 is 07 GPa. (b) The proportional limit is the stress level at which linearity of the stressstrain curve ends, which is approximately 300 MPa (43,500 psi). (c) The 0.00 strain offset line intersects the stressstrain curve at approximately 400 MPa (58,000 psi).
6 (d) The tensile strength (the maximum on the curve) is approximately 515 MPa (74,700 psi). 6.7 A load of 85,000 N (19,100 lb f ) is applied to a cylindrical specimen of a steel alloy (displaying the stress strain behavior shown in Figure 6.1) that has a crosssectional diameter of 15 mm (0.59 in.). (a) Will the specimen experience elastic and/or plastic deformation? Why? (b) If the original specimen length is 50 mm (10 in.), how much will it increase in length when this load is applied? This problem asks us to determine the deformation characteristics of a steel specimen, the stressstrain behavior for which is shown in Figure 6.1. (a) In order to ascertain whether the deformation is elastic or plastic, we must first compute the stress, then locate it on the stressstrain curve, and, finally, note whether this point is on the elastic or plastic region. Thus, from Equation 6.1 σ F A 0 85, 000 N π m N/m 481 MPa (69,900 psi) The 481 MPa point is beyond the linear portion of the curve, and, therefore, the deformation will be both elastic and plastic. (b) This portion of the problem asks us to compute the increase in specimen length. From the stressstrain curve, the strain at 481 MPa is approximately Thus, from Equation 6. l ε (0.0135)(50 mm) 3.4 mm (0.135 in.) 6.35 A cylindrical metal specimen having an original diameter of 1.8 mm (0.505 in.) and gauge length of mm (.000 in.) is pulled in tension until fracture occurs. The diameter at the point of fracture is 6.60 mm (0.60 in.), and the fractured gauge length is 7.14 mm (.840 in.). Calculate the ductility in terms of percent reduction in area and percent elongation.
7 This problem calls for the computation of ductility in both percent reduction in area and percent elongation. Percent reduction in area is computed using Equation 6.1 as %RA π d 0 π d f π d in which d 0 and d f are, respectively, the original and fracture crosssectional areas. Thus, %RA 1.8 mm π 6.60 mm π 1.8 mm π % While, for percent elongation, we use Equation 6.11 as %EL l f mm mm mm 100 4% Elastic Recovery After Plastic Deformation 6.49 A cylindrical specimen of a brass alloy 7.5 mm (0.30 in.) in diameter and 90.0 mm (3.54 in.) long is pulled in tension with a force of 6000 N (1350 lb f ); the force is subsequently released. (a) Compute the final length of the specimen at this time. The tensile stress strain behavior for this alloy is shown in Figure 6.1. (b) Compute the final specimen length when the load is increased to 16,500 N (3700 lb f ) and then released. (a) In order to determine the final length of the brass specimen when the load is released, it first becomes necessary to compute the applied stress using Equation 6.1; thus
8 σ F F A 0 π d N π m 136 MPa (19,000 psi) Upon locating this point on the stressstrain curve (Figure 6.1), we note that it is in the linear, elastic region; therefore, when the load is released the specimen will return to its original length of 90 mm (3.54 in.). (b) In this portion of the problem we are asked to calculate the final length, after load release, when the load is increased to 16,500 N (3700 lb f ). Again, computing the stress σ 16,500 N π m 373 MPa (5,300 psi) The point on the stressstrain curve corresponding to this stress is in the plastic region. We are able to estimate the amount of permanent strain by drawing a straight line parallel to the linear elastic region; this line intersects the strain axis at a strain of about 0.08 which is the amount of plastic strain. The final specimen length l i may be determined from a rearranged form of Equation 6. as l i (1 + ε) (90 mm)( ) 97.0 mm (3.8 in.)
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationSTANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius
MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationCHAPTER 7 MECHANICAL PROPERTIES PROBLEM SOLUTIONS
Excerpts from this work may be reproduced by instructors for distribution on a notforprofit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has
More information6.37 Determine the modulus of resilience for each of the following alloys:
6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationThe science of elasticity
The science of elasticity In 1676 Hooke realized that 1.Every kind of solid changes shape when a mechanical force acts on it. 2.It is this change of shape which enables the solid to supply the reaction
More informationN = N A Pb A Pb. = ln N Q v kt. = kt ln v N
5. Calculate the energy for vacancy formation in silver, given that the equilibrium number of vacancies at 800 C (1073 K) is 3.6 10 3 m 3. The atomic weight and density (at 800 C) for silver are, respectively,
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationSolid Mechanics Homework Answers
Name: Date: Solid Mechanics Homework nswers Please show all of your work, including which equations you are using, and circle your final answer. Be sure to include the units in your answers. 1. The yield
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationMATERIALS FOR CIVIL AND CONSTRUCTION ENGINEERS
MATERIALS FOR CIVIL AND CONSTRUCTION ENGINEERS 3 rd Edition Michael S. Mamlouk Arizona State University John P. Zaniewski West Virginia University Solution Manual FOREWORD This solution manual includes
More informationStress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus. Case study
Stress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus Case study 2 In field of Physics, it explains how an object deforms under an applied force Real rigid bodies are elastic we can
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationSolid Mechanics Chapter 1: Tension, Compression and Shear
Solid Mechanics Chapter 1: Tension, Compression and Shear Dr. Imran Latif Department of Civil and Environmental Engineering College of Engineering University of Nizwa (UoN) 1 Why do we study Mechanics
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationN = Shear stress / Shear strain
UNIT  I 1. What is meant by factor of safety? [A/M15] It is the ratio between ultimate stress to the working stress. Factor of safety = Ultimate stress Permissible stress 2. Define Resilience. [A/M15]
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationSTRESS, STRAIN AND DEFORMATION OF SOLIDS
VELAMMAL COLLEGE OF ENGINEERING AND TECHNOLOGY, MADURAI 625009 DEPARTMENT OF CIVIL ENGINEERING CE8301 STRENGTH OF MATERIALS I 
More informationPDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [ ] Introduction, Fundamentals of Statics
Page1 PDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [2910601] Introduction, Fundamentals of Statics 1. Differentiate between Scalar and Vector quantity. Write S.I.
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationFatigue Problems Solution
Fatigue Problems Solution Problem 1. (a) Given the values of σ m (7 MPa) and σ a (1 MPa) we are asked t o compute σ max and σ min. From Equation 1 Or, σ m σ max + σ min 7 MPa σ max + σ min 14 MPa Furthermore,
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More information12/8/2009. Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka
Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka Introduction and classes of properties Case studies showing selection of the right material for the job Deformation of material under the action of a
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More informationA concrete cylinder having a a diameter of of in. mm and elasticity. Stress and Strain: Stress and Strain: 0.
2011 earson Education, Inc., Upper Saddle River, NJ. ll rights reserved. This material is protected under all copyright laws as they currently 8 1. 3 1. concrete cylinder having a a diameter of of 6.00
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationELASTICITY (MDM 10203)
ELASTICITY () Lecture Module 3: Fundamental Stress and Strain University Tun Hussein Onn Malaysia Normal Stress inconstant stress distribution σ= dp da P = da A dimensional Area of σ and A σ A 3 dimensional
More informationCIVIL DEPARTMENT MECHANICS OF STRUCTURES ASSIGNMENT NO 1. Brach: CE YEAR:
MECHANICS OF STRUCTURES ASSIGNMENT NO 1 SEMESTER: V 1) Find the least moment of Inertia about the centroidal axes XX and YY of an unequal angle section 125 mm 75 mm 10 mm as shown in figure 2) Determine
More informationOutline. Organization. Stresses in Beams
Stresses in Beams B the end of this lesson, ou should be able to: Calculate the maimum stress in a beam undergoing a bending moment 1 Outline Curvature Normal Strain Normal Stress Neutral is Moment of
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationME 207 Material Science I
ME 207 Material Science I Chapter 3 Properties in Tension and Compression Dr. İbrahim H. Yılmaz http://web.adanabtu.edu.tr/iyilmaz Automotive Engineering Adana Science and Technology University Introduction
More informationFree Body Diagram: Solution: The maximum load which can be safely supported by EACH of the support members is: ANS: A =0.217 in 2
Problem 10.9 The angle β of the system in Problem 10.8 is 60. The bars are made of a material that will safely support a tensile normal stress of 8 ksi. Based on this criterion, if you want to design the
More information9 MECHANICAL PROPERTIES OF SOLIDS
9 MECHANICAL PROPERTIES OF SOLIDS Deforming force Deforming force is the force which changes the shape or size of a body. Restoring force Restoring force is the internal force developed inside the body
More informationThe objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties.
Objective: The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties. Introduction: Mechanical testing plays an important role
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationSean Carey Tafe No Lab Report: Hounsfield Tension Test
Sean Carey Tafe No. 366851615 Lab Report: Hounsfield Tension Test August 2012 The Hounsfield Tester The Hounsfield Tester can do a variety of tests on a small testpiece. It is mostly used for tensile
More informationMAAE 2202 A. Come to the PASS workshop with your mock exam complete. During the workshop you can work with other students to review your work.
It is most beneficial to you to write this mock final exam UNDER EXAM CONDITIONS. This means: Complete the exam in 3 hours. Work on your own. Keep your textbook closed. Attempt every question. After the
More information20. Rheology & Linear Elasticity
I Main Topics A Rheology: Macroscopic deformation behavior B Linear elasticity for homogeneous isotropic materials 10/29/18 GG303 1 Viscous (fluid) Behavior http://manoa.hawaii.edu/graduate/content/slidelava
More informationMECHANICS OF MATERIALS Sample Problem 4.2
Sample Problem 4. SOLUTON: Based on the cross section geometry, calculate the location of the section centroid and moment of inertia. ya ( + Y Ad ) A A castiron machine part is acted upon by a knm couple.
More informationISHIK UNIVERSITY DEPARTMENT OF MECHATRONICS ENGINEERING
ISHIK UNIVERSITY DEPARTMENT OF MECHATRONICS ENGINEERING QUESTION BANK FOR THE MECHANICS OF MATERIALSI 1. A rod 150 cm long and of diameter 2.0 cm is subjected to an axial pull of 20 kn. If the modulus
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationTheory at a Glance (for IES, GATE, PSU)
1. Stress and Strain Theory at a Glance (for IES, GATE, PSU) 1.1 Stress () When a material is subjected to an external force, a resisting force is set up within the component. The internal resistance force
More informationChapter Two: Mechanical Properties of materials
Chapter Two: Mechanical Properties of materials Time : 16 Hours An important consideration in the choice of a material is the way it behave when subjected to force. The mechanical properties of a material
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationElastic Properties of Solid Materials. Notes based on those by James Irvine at
Elastic Properties of Solid Materials Notes based on those by James Irvine at www.antonineeducation.co.uk Key Words Density, Elastic, Plastic, Stress, Strain, Young modulus We study how materials behave
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationCOMPLEX STRESS TUTORIAL 4 THEORIES OF FAILURE. You should judge your progress by completing the self assessment exercises.
COMPLEX STRESS TUTORIAL 4 THEORIES OF FAILURE This short tutorial covers no known elements of the E.C. or Edexcel Exams but should be studied as part of complex stress, structures and materials. You should
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationX has a higher value of the Young modulus. Y has a lower maximum tensile stress than X
Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which
More informationCHAPTER 9 FAILURE PROBLEM SOLUTIONS
Excerpts from this work may be reproduced by instructors for distribution on a notforprofit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has
More informationDate Submitted: 1/8/13 Section #4: T Instructor: Morgan DeLuca. Abstract
Lab Report #2: Poisson s Ratio Name: Sarah Brown Date Submitted: 1/8/13 Section #4: T 1012 Instructor: Morgan DeLuca Group Members: 1. Maura Chmielowiec 2. Travis Newberry 3. Thomas Cannon Title: Poisson
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: area (net with holes, bearing in contact, etc...) b total width of material at a horizontal section d diameter of a hole D symbol for diameter E modulus of elasticity
More informationJohns Hopkins University What is Engineering? M. Karweit MATERIALS
Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: MATERIALS A. Composition
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationStrength of Materials (15CV 32)
Strength of Materials (15CV 32) Module 1 : Simple Stresses and Strains Dr. H. Ananthan, Professor, VVIET,MYSURU 8/21/2017 Introduction, Definition and concept and of stress and strain. Hooke s law, StressStrain
More information(1) Brass, an alloy of copper and zinc, consists of 70% by volume of copper and 30% by volume of zinc.
PhysicsAndMathsTutor.com 1 Q1. (a) Define the density of a material....... (1) (b) Brass, an alloy of copper and zinc, consists of 70% by volume of copper and 30% by volume of zinc. density of copper =
More informationSolution: The strain in the bar is: ANS: E =6.37 GPa Poison s ration for the material is:
Problem 10.4 A prismatic bar with length L 6m and a circular cross section with diameter D 0.0 m is subjected to 0kN compressive forces at its ends. The length and diameter of the deformed bar are measured
More informationChapter 13 ELASTIC PROPERTIES OF MATERIALS
Physics Including Human Applications 280 Chapter 13 ELASTIC PROPERTIES OF MATERIALS GOALS When you have mastered the contents of this chapter, you will be able to achieve the following goals: Definitions
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationName :. Roll No. :... Invigilator s Signature :.. CS/B.TECH (CENEW)/SEM3/CE301/ SOLID MECHANICS
Name :. Roll No. :..... Invigilator s Signature :.. 2011 SOLID MECHANICS Time Allotted : 3 Hours Full Marks : 70 The figures in the margin indicate full marks. Candidates are required to give their answers
More informationSub. Code:
Important Instructions to examiners: ) The answers should be examined by key words and not as wordtoword as given in the model answer scheme. ) The model answer and the answer written by candidate may
More informationTENSILE TESTS (ASTM D 638, ISO
MODULE 4 The mechanical properties, among all the properties of plastic materials, are often the most important properties because virtually all service conditions and the majority of enduse applications
More informationExperiment Five (5) Principal of Stress and Strain
Experiment Five (5) Principal of Stress and Strain Introduction Objective: To determine principal stresses and strains in a beam made of aluminum and loaded as a cantilever, and compare them with theoretical
More informationLaboratory 7 Measurement on Strain & Force. Department of Mechanical and Aerospace Engineering University of California, San Diego MAE170
Laboratory 7 Measurement on Strain & Force Department of Mechanical and Aerospace Engineering University of California, San Diego MAE170 Megan Ong Diana Wu Wong B01 Tuesday 11am May 17 th, 2015 Abstract:
More informationElasticity. A PowerPoint Presentation by Paul E. Tippens, Professor of Physics Southern Polytechnic State University Modified by M.
Elasticity A PowerPoint Presentation by Paul E. Tippens, Professor of Physics Southern Polytechnic State University Modified by M. Lepore Elasticity Photo Vol. 10 PhotoDisk/Getty BUNGEE jumping utilizes
More informationMECE 3321: Mechanics of Solids Chapter 6
MECE 3321: Mechanics of Solids Chapter 6 Samantha Ramirez Beams Beams are long straight members that carry loads perpendicular to their longitudinal axis Beams are classified by the way they are supported
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationChapter 4b Axially Loaded Members
CIVL 222 STRENGTH OF MATERIALS Chapter 4b Axially Loaded Members AXIAL LOADED MEMBERS Today s Objectives: Students will be able to: a) Determine the elastic deformation of axially loaded member b) Apply
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationChapter kn m/kg Ans kn m/kg Ans. 187 kn m/kg Ans.
Chapter 1 From Tables A0, A1, A, and A4c, (a) UNS G1000 HR: S ut = 80 (55) MPa (kpsi), S yt = 10 (0) MPa (kpsi) Ans. (b) SAE 1050 CD: S ut = 690 (100) MPa (kpsi), S yt = 580 (84) MPa (kpsi) Ans. (c)
More information